| %Ge  | %As   | %S    | l 0 (nm) | T g (degC) | T s (degC) | a (ppm/degC) | r (g/cm3) | V (cm3) |
| 15   | 50    | 35    | 855      | 340        | 451        | 14.4         | 3.720     | 16.01   |
| 1.25 | 58.75 | 40    | 635      | 21         |            |              | 3.445     | 16.77   |
| 2.5  | 57.5  | 40    |          | 40         |            |              |           |         |
| 5    | 55    | 40    |          | 192        |            |              |           |         |
| 7.5  | 52.5  | 40    | 683      | 202        | 329        | 40.5         | 3.518     | 16.38   |
| 10   | 50    | 40    | 723      | 267        | 383        | 28.9         | 3.533     | 16.29   |
| 15   | 45    | 40    | 728      | 321        | 435        | 17.8         | 3.559     | 16.14   |
| 1.25 | 56.25 | 42.5  | 650      | 30         | 49         |              | 3.473     | 16.32   |
| 2.5  | 55    | 42.5  | 671      | 42         | 85         |              | 3.489     | 16.24   |
| 5    | 52.5  | 42.5  |          |            |            |              | 3.433     | 16.49   |
| 1.25 | 53.75 | 45    |          | 14         |            |              | 3.400     | 16.35   |
| 5    | 50    | 45    |          | 51         |            |              | 3.424     | 16.21   |
| 10   | 45    | 45    | 691      |            | 341        | 40.5         | 3.388     | 16.35   |
| 15   | 40    | 45    | 799      | 298        | 420        | 22.7         | 3.401     | 16.26   |
| 2.5  | 51.25 | 46.25 | 595      | 34         | 49         |              | 3.391     | 16.23   |

Caption: Physical properties of As-rich, S-deficient glasses

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "15", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "35", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "855", "type": "Other"}
{"value": "340", "type": "Other"}
{"value": "451", "type": "Other"}
{"value": "14.4", "type": "Other"}
{"value": "3.720", "type": "Other"}
{"value": "16.01", "type": "Other"}
{"value": "1.25", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "58.75", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "635", "type": "Other"}
{"value": "21", "type": "Other"}
{"value": "3.445", "type": "Other"}
{"value": "16.77", "type": "Other"}
{"value": "2.5", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "57.5", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "40", "type": "Other"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "55", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "192", "type": "Other"}
{"value": "7.5", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "52.5", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "683", "type": "Other"}
{"value": "202", "type": "Other"}
{"value": "329", "type": "Other"}
{"value": "40.5", "type": "Other"}
{"value": "3.518", "type": "Other"}
{"value": "16.38", "type": "Other"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "723", "type": "Other"}
{"value": "267", "type": "Other"}
{"value": "383", "type": "Other"}
{"value": "28.9", "type": "Other"}
{"value": "3.533", "type": "Other"}
{"value": "16.29", "type": "Other"}
{"value": "15", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "728", "type": "Other"}
{"value": "321", "type": "Other"}
{"value": "435", "type": "Other"}
{"value": "17.8", "type": "Other"}
{"value": "3.559", "type": "Other"}
{"value": "16.14", "type": "Other"}
{"value": "1.25", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "56.25", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "42.5", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "650", "type": "Other"}
{"value": "30", "type": "Other"}
{"value": "49", "type": "Other"}
{"value": "3.473", "type": "Other"}
{"value": "16.32", "type": "Other"}
{"value": "2.5", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "55", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "42.5", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "671", "type": "Other"}
{"value": "42", "type": "Other"}
{"value": "85", "type": "Other"}
{"value": "3.489", "type": "Other"}
{"value": "16.24", "type": "Other"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "52.5", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "42.5", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "3.433", "type": "Other"}
{"value": "16.49", "type": "Other"}
{"value": "1.25", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "53.75", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "14", "type": "Other"}
{"value": "3.400", "type": "Other"}
{"value": "16.35", "type": "Other"}
{"value": "5", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "50", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "51", "type": "Other"}
{"value": "3.424", "type": "Other"}
{"value": "16.21", "type": "Other"}
{"value": "10", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "691", "type": "Other"}
{"value": "341", "type": "Other"}
{"value": "40.5", "type": "Other"}
{"value": "3.388", "type": "Other"}
{"value": "16.35", "type": "Other"}
{"value": "15", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "40", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "45", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "799", "type": "Other"}
{"value": "298", "type": "Other"}
{"value": "420", "type": "Other"}
{"value": "22.7", "type": "Other"}
{"value": "3.401", "type": "Other"}
{"value": "16.26", "type": "Other"}
{"value": "2.5", "type": "Glass_Compound_Amount", "constituent": "Ge", "unit": "mol", "material": "xx"}
{"value": "51.25", "type": "Glass_Compound_Amount", "constituent": "As", "unit": "mol", "material": "xx"}
{"value": "46.25", "type": "Glass_Compound_Amount", "constituent": "S", "unit": "mol", "material": "xx"}
{"value": "595", "type": "Other"}
{"value": "34", "type": "Other"}
{"value": "49", "type": "Other"}
{"value": "3.391", "type": "Other"}
{"value": "16.23", "type": "Other"}